Direct Electroplated Metallization on Indium Tin Oxide Plastic Substrate Nga Yu Hau,†,§ Ya-Huei Chang,†,§ Yu-Ting Huang,† Tzu-Chien Wei,‡ and Shien-Ping Feng*,† †
Department of Mechanical Engineering, The University of Hong Kong, Pokfulam, Hong Kong Department of Chemical Engineering, National Tsing-Hua University, Hsinchu, Taiwan
S Supporting Information *
ABSTRACT: Looking foward to the future where the device becomes ﬂexible and rollable, indium tin oxide (ITO) fabricated on the plastic substrate becomes indispensable. Metallization on the ITO plastic substrate is an essential and required process. Electroplating is a cost-eﬀective and high-throughput metallization process; however, the poor surface coverage and interfacial adhesion between electroplated metal and ITO plastic substrate limits its applications. This paper develops a new method to directly electroplate metals having strong adhesion and uniform deposition on an ITO plastic substrate by using a combination of 3mercaptopropyl-trimethoxysilane (MPS) self-assembled monolayers (SAMs) and a sweeping potential technique. An impedance capacitive analysis supports the proposed bridging link model for MPS SAMs at the interface between the ITO and the electrolyte.
1. INTRODUCTION Indium tin oxide (ITO) having superior optical and electrical properties has been widely fabricated on glass as a substrate in optoelectronic applications, such as thin-ﬁlm transistors, ﬂat panel displays, light-emitting diodes (LED), optical sensors, electrochromic windows, and photovoltaic cells. Thermal evaporation, pulsed-laser deposition and sputtering techniques are the most common methods to fabricate transparent conducting ITO thin ﬁlms (150−200 nm) on glass substrates at a temperature of 300−350 °C.1,2 Metallization on ITO substrate is crucial to various purposes in devices, such as silver interconnects for device-to-device integration, gold current collectors in optical sensors, and platinum counter electrodes in dye-sensitized solar cells.3−6 It is relatively common to screenprint a metal over ITO surface with a conductive paste. After burning out polymer binders by postannealing at a temperature of 200−500 °C, a conductive metal layer can be formed on the ITO surface. Toward the future where the device goes ﬂexible and rollable, ITO fabricated on a plastic substrate becomes indispensable. Contrary to the rigid glass, the polymeric substrates, such as polyethylene naphthalate (PEN) or poly(ethylene terephthalate)(PET), cannot withstand the high temperature so that ITO has to be coated by using rf or dc magnetron sputtering at low temperature (